Kent D. Peaslee Steel Manufacturing Research Center
Missouri University of Science & Technology
Evolution of Non-Metallic Inclusions in Foundry Steel Casting
Marc Harris Dr. Von L. Richards Dr. Ron O’Malley Dr. Simon
SFSA Technical and Operating Conference, December 2015
Evolution of Non-Metallic Inclusions in Foundry Steel Casting
Missouri University of Science & Technology
Marc Harris Dr. Von L. Richards Dr. Ron O’Malley Dr. Simon
The evolution of nonmetallic inclusions was examined for 4320
steel at an industrial steel foundry. The steel was followed from
electric arc furnace melting through ladle refining to final
casting. Timed sampling was performed at all stages of the process.
Samples were analyzed using an automated SEM/EDS system. The
overall evolution of oxide inclusions in terms of nucleation,
growth, and flotation during liquid processing was studied using
area fraction and average diameter. Chemical composition evolution
was observed using a joint ternary plotting tool developed under
this program. It was found that the use of zirconium as an addition
for nitrogen/oxygen removal leads to a large number of ZrO2
inclusions, which is related to insufficient flotation due to the
higher density of zirconia and in turn less effective calcium
treatment. In addition, no ZrN formation was observed, likely due
to the high FeO acid slag practice used. Argon stirring was found
to reduce the flotation problems associated with the zirconium
addition somewhat and significantly contribute to the removal of
large size (>5µm) inclusions.
Steel cleanliness is of increasing interest as demand increases
for high quality, clean steel castings. Mechanical properties are
affected by inclusion size, number, and morphology. Therefore
research is being conducted to improve inclusion control thus
minimizing the detrimental effects of inclusions on final
properties. The evolution of nonmetallic inclusions throughout the
production process must first be understood and controlled in order
to control the final inclusion population.
Nonmetallic inclusions can be formed in the melt and upon
solidification (indigenous) by exceeding the solubility limits of
inclusion forming reactants in the liquid or can be introduced by
external contamination events (exogenous). The most common source
of nonmetallic inclusions is from melt reactions with dissolved
oxygen. Typically, for steel castings, porosity is considered
highly detrimental and the most common method to eliminate gas (CO)
porosity is the use of deoxidizers (usually aluminum or silicon).
This is an effective method of deoxidation, but it results in the
generation of a large oxide inclusion population. These oxides can
be highly problematic for certain steel grades where there are
stringent specifications, having negative effects on castability,
mechanical properties, and compliance with cleanliness
Current theories about the evolution of nonmetallic inclusions
normally include the following stages: (i) nucleation, (ii)
growth/agglomeration, and (iii) flotation[1-2]. A review of
state-of-the-art theories of liquid steel refining in large scale
metallurgical ladles was recently published by Zhang and Thomas.
Inclusion nucleation requires chemical supersaturation which is
affected by the chemical affinity of active elements to
non-metal impurities (S, O, N) in solution in the melt, as well
as alloy composition, temperature, and other factors. Nucleation
is largely understood based on surface energy minimization such
that above some critical radius, a stable nucleus is successfully
formed and subsequently grows. This growth will spontaneously occur
when the critical radii of the nuclei are exceeded. Inclusion
nucleation requires chemical supersaturation which is affected by
alloy composition, additions, temperature, and other
After nucleation, growth of a nonmetallic inclusion occurs
through a variety of mechanisms, with the key phenomenon being
Ostwald ripening driven by diffusion of elements and local
thermodynamics. Growth by agglomeration has also been considered.
For sub-micron particles the contacting mechanism for agglomeration
is currently thought to be the result of Brownian collision.
Somewhat larger particles however, are more affected by melt flow
such as turbulent collision or differential flotation velocities
according to Stoke’s Law[1-2]. This agglomeration process, in the
case of Al2O3, is more efficient when the inclusions are in the
liquid state which is one goal of CaSi modification treatments. The
calcium in this case leads to the formation of a CaO·Al2O3 liquid
state inclusion that is both spherical and has increased tendency
to agglomerate, increasing flotation velocity[1-4].
Flotation is best described by Stokes’ Law for unstirred systems
where the velocity of a particle is dependent on the density
differential and its size according to Equation 1:
where: vs is the particle velocity, ρp is the particle density,
ρf is the fluid density, g is the gravitational constant, and R is
the particle radius. Stirring with argon gas is used to aid in
inclusion flotation in the ladle. The gas enters through an
eccentrically located porous plug in the ladle bottom. The stirring
results in reduced content of large sized inclusions. The stirring
increases net flotation by both increasing overall fluid velocity,
and through inclusion wetting and attachment to the bubble itself,
which typically results in reduced content of large sized
The theories discussed here are well known and supported through
countless experiments, but all three basic phenomena
(nucleation-growth-flotation) occur simultaneously in liquid steel
processing which complicates the study of nonmetallic
inclusions[1-2]. It is important to consider that these mechanisms
are interrelated and occurring the entire time the steel is in the
liquid state. As time progresses the nucleated inclusion
populations in the melt are expected to grow in size according to
the prevailing growth mechanism, and enlarged particles have
increased flotation velocity. Understanding the overall evolution
of inclusions throughout liquid steel refining processes is
critical in order to control final product cleanliness[6-7].
Recently, work has been done on the evolution of inclusions in
continuous casting steelmaking processes applying an automated
SEM-EDS system. This method allows for one to obtain important
compositional data with statistical significance when examining
such large volumes of production[10-18]. The formation of
inclusions in a steel mill can be more controlled with limited
oxygen exposure, narrow ranges of alloying, and consistent product
geometry and size. These restrictions are often infeasible for
foundries where castings are complex and variable. Work by Singh et
al. examined four foundry processes using an automated SEM-EDS
system and reviewed the effectiveness of calcium treatments on the
inclusion population as well as discussing optimum treatments.
In the present study, a similar approach is used to both evaluate
the deoxidation practice, the calcium treatment effectiveness
in relation to the deoxidation practice, the effect of argon
stirring, and to understand the overall evolution of inclusions in
the steel foundry processing route for carbon and low alloy steel
Industrial Process Sampling
A comprehensive study of steel melt processing at an industrial
foundry was performed for three heats (melt through casting).
Sampling points for the foundry can be seen in Figure 1 along with
an outline of the processing steps at each sampling point, a
schematic overview of the process including ladle design, as well
as the time at which the samples were taken. The three heats which
were sampled include: an aluminum/zirconium deoxidized heat (Heat
AA), an aluminum deoxidized heat (Heat B), and an
aluminum/zirconium deoxidized heat that employed argon stirring
(Heat C). Heats AA and B were not argon stirred. The foundry melts
were produced in a 5 ton EAF and poured using a stopper rod
bottom-pour ladle. The steel was deoxidized with aluminum or
aluminum and zirconium and a calcium treatment was performed using
wire injection with steel jacketed CaSi wire. The calcium levels
obtained in each heat after the CaSi wire treatment is given in
Table 1. The reported final chemistries (via arc spectroscopy) for
each heat can is presented in Table 2.
Figure 1. Schematic of three sampled heats (designated AA, B,
and C) with process variations and sample locations shown.
Table 1. Calcium content (wt%) after CaSi wire injection.
Ca (wt%) Heat AA 0.019 Heat B 0.025 Heat C 0.024
Table 2. Steel chemistry (wt %) measured via arc
C Si Mn P Cr Mo Ni Al Co Cu V Fe 0.25 ± .043
0.52 ± .011
0.80 ± .028
0.025 ± .00005
0.76 ± .040
0.37 ± .011
1.11 ± .037
0.064 ± .013
0.013 ± .00055
0.093 ± .011
0.055 ± .008 bal.
Samples taken in the EAF and ladle prior to casting were
unkilled steel chilled immersion samples taken from the top of the
melt. The in-stream specimens were acquired from the liquid stream
during the casting process (bottom of the ladle). The shape and
sectioning method of the samples can be seen in Figure 2. The
center sectioning method was used in order to minimize
contamination effects, such as scale or slag entrainment that can
occur at the surface. Specimens were ground using SiC media (180,
400, 600, 1200 grits), polished using 3µm diamond paste, and
finished using a 0.1µm diamond paste. Metallographic preparation
was done in accordance to ASTM E3-11 for all samples.
Figure 2. Sample sectioning method used for automated SEM/EDS
After preparation, samples were scanned using an automated ASPEX
SEM/EDS system. Scans were performed using a 0.5µm minimum
inclusion diameter threshold (limit of instrument), medium scan
speed, 20 keV accelerating voltage, and a nominal EDS detection
time of 1 second (Table 3). The step size of the search grid was
0.16µm which allows 100% detection of inclusions as small as 0.5µm
in diameter. Porosity was excluded from consideration using an
EDS minimum count threshold of 1000, an example of which is shown
in Figure 3 where a large region of porosity has been excluded from
the analysis due to low counts.
Table 3. ASPEX SEM/EDS settings used in the analysis.
Exclusion Rules Mag.
Minimum Diameter Threshold
Max Particle Count
20 keV 40-50 !A 1 second Mg, Al, Si, Zr, S, Ca, Ti, Mn > 1000
0.16 !m 0.5 !m 2500 8%
Figure 3. Large region of porosity with low counts per second
(CPS) that leads to exclusion from analysis.
Automated analysis provides an averaged EDS spectrum near the
inclusion center. In the case of complex or agglomerated inclusion
types an additional post-processing filter was applied. The goal of
this filtering was de-selection of sulfides from oxides through
applying a sulfur concentration threshold (greater than 30% S). The
statistical basis of this procedure is given in Harris et
al.!This technique allows the monitoring of Al2O3 modification
as well as general oxide modification.
A method of calculating a mass balance from SEM-EDS data was
used that allows the study of elemental content contained within
inclusions. The areal average elemental composition of inclusions
is calculated for each element as follows:
!! ! !! !!!"#$%&!'"!!!"!#$
where: %m is the areal average mass percent of a given element,
%x is the amount of respective element in an individual inclusion,
Ainclusion and Atotal are the area of the individual inclusion and
total area of all measured inclusions. The mass balance calculation
was performed using the compositional data obtained from the
SEM-EDS inclusion analysis and Equation 3:
!!!" ! !!!!!!!!!!!!
where: Mppm is the mass fraction in ppm of a given element in a
sample contained within inclusions, %m is the areal average mass
percent of a given element, Af is the total inclusion area
fraction, !i and !m are the density of the inclusion associated
with the given element and the density of the matrix respectively
(taken to be iron), and wi is the mass fraction of the given
element in the associated inclusion compound.
The oxide area fraction was examined closely for Heat AA, Heat
B, and Heat C and is summarized in Figure 4. The behavior of three
size classes of inclusions is shown for each liquid processing
stage where these heats were compared for the purpose of
determining the effectiveness of argon stirring practice and
zirconium additions as a nitrogen/oxygen gettering treatment. A
cut-off of 5 micron was somewhat arbitrarily used for the “large”
size fraction since the 5 micron and above inclusions seemed to
behave differently in terms of floatation in this industrial
process. It was observed that with the addition of zirconium, the
total oxide area fraction of inclusions grows with time in the
ladle and that, concurrently, the inclusion size distribution
shifts to larger diameters. The opposite is true when only aluminum
is used. In this case, the inclusion population shifts from large
area fraction with coarse particles to a finer size distribution
and a lower area fraction with time in the ladle.
Figure 4. Oxide area fraction for three size ranges across a)
Heat AA, b) Heat B, and c) Heat C.
The difference in behavior of the inclusion population with time
in Heat AA and Heat B (Figure 5) appears to result from the
difference in deoxidation practice used and its effect on inclusion
flotation. Each melt was poured into 7 molds of known weight while
in-stream sampling was performed from the pouring stream below the
bottom of the ladle. Different molds in the sequence represent
different melt levels in the ladle, where the first mold is from
the bottom region of the ladle, and the last mold is near the top
region. In Heat B (Al killed), the oxide area fraction was found to
decrease going from the bottom of the ladle to the top over a time
interval of eight minutes. In the case of Heat AA (Al+Zr killed),
the opposite was found to be true: the oxide area fraction
increased going from the bottom of the melt to the top. The upper
quarter of the ladle appeared to accumulate an increased area
fraction of inclusions compared to the bottom quarter of the ladle
(450 ppm compared to 250 ppm) over a time interval of twelve
minutes. By comparison, Heat B showed a drop from 700 ppm to 400
ppm oxide area fraction. Heat C, which was argon stirred, retained
a uniform low level of oxide area fraction (400-450 ppm) throughout
Figure 5. Oxide area fraction as a function of melt level for
In order to better understand the difference in treatment
practice a mass balance calculation based on Eq. 2 was performed
for four elements: aluminum, silicon, zirconium, and calcium
(Figure 6). It was also found that the content (mass ppm) of
aluminum in the samples in the form of inclusions increased
immediately after deoxidation in all heats before decreasing as a
result of inclusion removal. The content of silicon in inclusions
decreased after deoxidation indicating that the population of
silicates was reduced by the more thermodynamically stable Al2O3
and/or ZrO2 according to Eq. 4 and Eq. 5:
3SiO2 + 4[Al] = 2Al2O3 + 3[Si] (4)
[Zr] + SiO2 = ZrO2 + [Si] (5)
The mass of zirconium reacted to form inclusions increased only
after deoxidation in Heat AA and Heat C where zirconium was
Figure 6. Changing total concentration of active elements within
inclusions during ladle processing of analyzed heats: a) Al, b) Si,
c) Zr, and d) Ca.
Calcium levels for each heat after CaSi treatment are presented
in Table 1. The calcium content of inclusions increased in all
heats after the treatment. However, Heat AA retained a lower mass
ppm of calcium in the modified inclusions and had a lower final
calcium to aluminum ratio (approx. 0.16) than that of Heat B
(approx. 0.28). The slag compositions for each sampling are
presented in Table 4 and an overview of the composition of the
inclusion population (Figure 7) shows the progression of the
inclusions for the different deoxidation practices. The composition
of the oxide inclusion population after calcium addition for Heat
AA can be seen to include a large number of ZrO2 rich inclusions
containing some calcium. In Heat B, very little ZrO2 is present and
most of the population is close to the liquid phase field of the
CaO"Al2O3 binary system.
Table 4. Slag chemistries in wt. % of all heats at various
liquid process stages.
%SiO2 %CaO %MgO %Al2O3 %TiO2 %Fe2O3 %MnO2 %ZrO2 %C
Heat AA EAF
After Melt Down 50.29 2.91 0.19 8.89 0.39 8.40 29.67 0.82 0.03
After 1st O2 Blow 50.11 2.14 0.14 7.31 0.34 10.71 28.69 0.60
After Block 48.83 2.03 0.16 6.93 0.33 9.30 33.31 0.53 0.17
Ladle After Tap/Kill 52.04 1.86 0.18 8.16 0.33 6.81 31.13 0.69
0.00 After CaSi 49.25 2.13 0.18 9.28 0.36 6.66 32.71 0.86 0.02
Heat B EAF After Melt Down 51.72 2.20 0.26 6.27 0.31 18.21 20.13
0.21 0.06 After Block 52.91 1.43 0.15 5.85 0.34 11.30 28.38 0.16
Ladle After Tap/Kill 51.80 1.41 0.18 8.01 0.34 8.45 30.50 0.18
0.05 After CaSi 51.48 1.71 0.17 8.92 0.35 7.78 30.47 0.20 0.02
After Melt Down 58.67 3.68 0.17 4.59 0.34 10.67 21.34 0.12 0.03
After 1st O2 Blow 54.98 3.16 0.21 4.82 0.35 11.73 24.39 0.11 0.03
After 2nd O2 Blow 54.42 2.69 0.16 4.79 0.33 13.42 23.04 0.11
After Block 55.04 2.15 0.18 5.26 0.36 12.34 24.72 0.09 0.03
LadleAfter Tap/Kill 52.69 2.05 0.19 8.21 0.36 8.73 28.69 0.26
After CaSi 52.05 2.34 0.18 8.71 0.38 7.74 28.93 0.61 0.00After
Ar Stop 52.08 2.30 0.18 8.92 0.38 7.58 29.11 0.59 0.04
Figure 7. Joint ternary diagrams for a) Heat AA after
deoxidation, b) Heat B after deoxidation, c) Heat AA after calcium
treatment, d) Heat B after calcium treatment.
Measurements of total oxygen obtained by the inert gas fusion
method were compared to calculated mass ppm of oxygen in the oxide
inclusions that was obtained from SEM/EDS data. A linear
relationship was found (Figure 8), which suggests that most of the
oxygen in the steel is present in the form of oxide inclusions.
Figure 9, where t=0 is directly after melt down, shows that total
oxygen decreases with time after the completion of oxygen blowing
in the melt. This indicates that oxygen is being removed from the
system. This suggests that the inclusions are being removed by
Figure 8. Linear relationship between oxide area fraction and
total oxygen measured via inert gas fusion.
Figure 9. Decreasing total oxygen as a function of liquid
processing time for aluminum and aluminum/zirconium treated
The oxide inclusion area fraction decreased with ladle
processing time after initial deoxidizing additions, which is also
consistent with flotation as the mechanism for oxygen removal
(Figure 10). The flotation velocity is well understood from Stoke’s
Law to be a function of the particle size and density. Thus
inclusion growth plays a key role in the removal process. The
growth of inclusions can be seen more directly by examining the
average inclusion diameter in Figure 11 where the zero time is just
before tapping and deoxidation. An initial decrease in size as a
result of ladle deoxidation additions that nucleate large
populations of small (
Figure 11. Reduction in inclusion size during deoxidation stages
(nucleation) followed by a growth stage.
Deoxidation practice has a large effect on non-metallic
inclusion evolution during processing. The composition change of
the oxide inclusion population with time in the joint ternary plot
(Figure 7) shows the effectiveness of deoxidizing method and
modification clearly. The density of the type of oxide formed
affects flotation. In the case of the aluminum deoxidized system,
Al2O3 was formed which has a density of approximately 4 g/cm# while
the aluminum-zirconium treated heat formed ZrO2 with a density of
approximately 5.7 g/cm#. This density difference leads to a slower
flotation rate for ZrO2 rich inclusions which results in an
increase in oxide area fraction at the top region of the ladle when
compared to the aluminum killed heat. The Al2O3 is more quickly
removed from the system as a result of its low density and the
effect of calcium treatment aimed at forming liquid CaO"Al2O3 which
speeds flotation further. This faster removal rate leads to a more
homogenous melt and a decrease in oxide area fraction over the time
span from treatment through pouring the last production casting
from the ladle. The use of argon stirring in the aluminum-zirconium
treated heat (Heat C) aided the homogenization of the heat and
helped mitigate the build-up of oxides in the top region of the
melt by assisting inclusion flotation. It is important to note that
the addition of zirconium was also expected to act as a nitrogen
getter but no ZrN was observed in any samples. This may only be
true because of the high oxygen potential of the 7-8% FeO and
29-32% MnO content of the ladle slag (Table 4) that was employed.
The nitrogen content for Heat AA was notably high at approximately
500 ppm but still no ZrN formed (Figure 12).
Figure 12. Total nitrogen content measured using inert gas
fusion at each sampling point for all heats.
Three industrial 4320 steel heats were followed from melting to
ladle pouring in an effort to develop an understanding of the
evolution of nonmetallic inclusions through a typical steel foundry
process. Immersion sampling was performed at various stages during
liquid steel processing in an operating industrial foundry. Three
heats with different steelmaking practices were compared: (1)
aluminum deoxidized, calcium treated; (2) aluminum/zirconium
deoxidized, calcium treated; and (3) aluminum/zirconium deoxidized,
calcium treated, argon stirred (Heats AA, B, and C respectively).
In order to effectively analyze the evolution of large populations
of inclusions, an automated SEM-EDS system was used which enabled a
statistically significant number of nonmetallic inclusions to be
The aluminum-zirconium treated heats had a lower calcium
recovery and exhibited a slower rate of inclusion flotation because
of the higher density of ZrO2 inclusions compared to the Al2O3
inclusions generated in an aluminum killed heat. Argon stirring was
found to aid in the removal of large sized (> 5µm) inclusions in
an aluminum-zirconium treated heat, but had little effect on the
inclusion composition. It was noted that using argon stirring in
conjunction with an aluminum-zirconium killing practice helped to
increase the inclusion flotation rate compared to
aluminum-zirconium killing without argon stirring.
1. Zhang, Lifeng, and Brian Thomas. "Inclusion Nucleation,
Growth, and Mixing During Steel Deoxidation." Continuous Casting
2. Deng, Zhiyin, and Miaoyong Zhu. "Evolution Mechanism of
Non-metallic Inclusions in Al-Killed Alloyed Steel during Secondary
Refining Process." ISIJ International 53: 450-458.
3. Higuchi, Yoshihiko, Mitsuhiro Numata, Shin Fukagawa, and
Kaoru Shinme. "Inclusion Modification by Calcium Treatment." ISIJ
International 36: 151-154.
4. Yang, Wen, Lifeng Zhang, Xinhua Wang, Ying Ren, Xuefeng Liu,
and Qinglin Shan. "Characteristics of Inclusions in Low Carbon
Al-Killed Steel during Ladle Furnace Refining and Calcium
Treatment." ISIJ International 53: 1401-1410.
5. Van Ende, Marie-Aline, Muxing Guo, Joris Proost, Bart
Blanpain, and Patrick Wollants. "Formation and Morphology of Al2O3
Inclusions at the Onset of Liquid Fe Deoxidation by Al Addition."
ISIJ International 51: 27-34.
6. Verma, Neerav, Petrus Pistorius, Richard Fruehan, Michael
Potter, Minna Lind, and Scott Story. "Transient Inclusion Evolution
During Modification of Alumina Inclusions by Calcium in Liquid
Steel: Part I. Background, Experimental Techniques, and Analysis
Methods." Metallurgical and Materials Transactions B:v42(4):
7. Verma, N., Petrus Pistorius, Richard Fruehan, Michael Potter,
Minna Lind, and Scott Story. "Transient Inclusion Evolution During
Modification of Alumina Inclusions by Calcium in Liquid Steel: Part
II. Results and Discussion." Metallurgical and Materials
Transactions B: v42(4):720-729.
8. Holappa, L.. "On Physico-Chemical and Technical Limits in
Clean Steel Production." Steel Research International 81:
9. Lou, Wentao, and Miaoyong Zhu. "Numerical Simulations of
Inclusion Behavior in Gas-Stirred Ladles." Metallurgical and
Materials Transactions B 44B: 762-782.
10. Singh, Vintee, Kent Peaslee, and Simon Lekakh. "Use of
Automated Inclusion Analysis to Evaluate the Effects of Ladle
Treatment on Steel Cleanliness."63rd SFSA T&O.
11. Singh, Vintee, Simon Lekakh, and Kent Peaslee. "Using
Automated Inclusion Analysis for Casting Process Improvements."
63rd SFSA T&O.
12. Michelic, Susanne, Gerhard Wieser, and Christian Bernhard.
"On the Representativeness of Automated SEM/EDS Analyses for
Inclusion Characterisation with Special Regard to the Measured
Sample Area." ISIJ International 51: 769-775.
13. Singh, Vintee, Simon Lekakh, Timothy Drake, and Kent
Peaslee. "Process Design of Inclusion Modification in Cast Steel
using Automated Inclusion Analysis."2009. 1-11.
14. Zhang, Zhi, Anders Tilliander, Andrey Karasev, and Par
Jonsson. "Simulation of the Steel Sampling Process." ISIJ
International 50: 1746-1755.
15. Kawakami, Masahiro, Eiji Nakamura, Shuzou Matsumoto, and
Seiji Yokoyama. "Morphological Classification of Inclusions in
Steel by Image Processing of Micrograph."ISIJ International 36:
16. Abraham, Sunday, Justin Raines, and Rick Bodnar.
"Development of an Inclusion Characterization Methodology for
Improving Steel Product Cleanliness."2013. 1069-1083.
17. Kaushik, P., H. Pielet, and H. Yin. "Inclusion
characterisation – tool for measurement of steel cleanliness and
process control: Part 1." Ironmaking and Steelmaking 36:
18. Kaushik, P., H. Pielet, and H. Yin. "Inclusion
characterisation – tool for measurement of steel cleanliness and
process control: Part 2."Ironmaking and Steelmaking36: 572-582.
19. Harris, Marc, Obinna Adaba, Simon Lekakh, Ron O'Malley, and
Von Richards. "Improved Methodology for Automated SEM/EDS
Non-Metallic Inclusion Analysis of Mini-Mill and Foundry Steels."
AISTech 2015 Proceedings 2015 (2015). Print.